Loading in 5 sec....

Energy Bands and III-V AlloysPowerPoint Presentation

Energy Bands and III-V Alloys

- 499 Views
- Uploaded on

Download Presentation
## PowerPoint Slideshow about 'Energy Bands and III-V Alloys' - LionelDale

**An Image/Link below is provided (as is) to download presentation**

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Presentation Transcript

### Energy Bands and III-V Alloys

EP 4E03 – September 19, 2006

{Streetman Section 3.1, with emphasis on 3.1.5}

Goals

- Review, in a qualitative manner, the underlying principles of energy bands in solids;
- Discuss the importance of III-V materials:
- Introduction to various alloys,
- Main applications,
- Design considerations.

Note:This presentation does not strictly follow Streetman’s treatment, but instead introduces the topics in a different manner. Moreover, a wider coverage of the important III-V materials is provided.

In the solid, the separation between the constituting atoms is comparable to the atomic size, so the properties of the individual atoms are altered by the presence of neighbouring atoms.

Review of Energy Bands (1)In crystalline solids, the atoms are “assembled” in a periodical arrangement, in such a way as to minimize the energy of the system…

Example: NaCl crystal (ionic bound)

Kasap, S.O., Principles of electrical engineering materials and devices, McGraw-Hill, 1997

Since the solid is made of a very large number of atoms (N), these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).

Review of Energy Bands (2)Holden A., The nature of solids, Dover Publications, 1965

The permitted energies that an electron can occupy in the isolated atoms are split into energy bands as the atoms get closer to each other.

This can also be visualized in terms of an overlap of the electron wave functions (Streetman section 3.1.2).

Outer shell

a + b these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).

e.g. a 1-D crystal could for instance be represented in the following manner:

Uo

a

Adapted from: R. Eisberg, R. Resnick, Quantum physics of atoms, molecules, solids, nuclei, and particles (2nd ed.), Wiley, 1985

b

a + b

x = 0

Review of Energy Bands (3)Mathematically, it means solving the time-independent Schrödinger’s equation:

where U(r) is the periodic effective potential energy that describes the arrangement of atoms in the crystal.

Actual band diagram these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).

For device description a much more simple and practical representation is typically used:

Eg ~ 1.4 eV

Ec

Eg

Ev

Cohen M.L., Chelikowski, J.R., Electronic Structure and Optical Properties of semiconductors, Springer, 1989

Review of Energy Bands (4)The solution to the equation is usually given in the form of a “band diagram” E vs k.

Yu, P.Y., Cardona, M., Fundamentals of semiconductors, Springer, 2005

e.g.GaAs crystal

Review of Energy Bands (5) these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).

Direct band gap semiconductors (e.g. GaAs, InP, InAs, GaSb)

The minimum of the conduction band occurs at the same k value as the valence band maximum.

Eg ~ 1.4 eV

Cohen M.L., Chelikowski, J.R., Electronic Structure and Optical Properties of semiconductors, Springer, 1989

Review of Energy Bands (6) these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).

Indirect band gap semiconductors (e.g. Si, Ge, AlAs, GaP, AlSb)

The minimum of the conduction band does not occur at the same k value as the valence band maximum.

An electron promoted to the conduction band requires a change of its momentum to make the transition to the valence band (typ. occurs via lattice vibrations).

Eg ~ 2.3 eV

Cohen M.L., Chelikowski, J.R., Electronic Structure and Optical Properties of semiconductors, Springer, 1989

III-V Materials these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).

Binary Compounds

III

IV

V

- Arsenides: GaAs, AlAs, InAs
- Phosphides: GaP, AlP, InP
- Antimonides: GaSb, AlSb, InSb
- Nitrides: GaN, AlN, InN

Tu, K-N, Mayer, J.W, Feldman, L.C., Electronic thin film science for electrical engineers and materials scientists, McMillan, 1992

Why III-V’s for devices? these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).

- Very low effective mass compared to Si (e.g. m*nl,Si = 0.98mo, m*n,GaAs = 0.067mo, m*n,InSb = 0.014mo):
- This translates into very high electron mobilities for high-speed electronic applications.

- A wide variety of these materials have a direct band gap:
- Photon emission is most efficient during recombination processes, so very suitable for light sources (lasers, LED’s), but also detectors.

- Possibility to create alloys consisting of the different elements:
- The properties of the device (e.g. emission wavelength of a light source) can be tailored to suit the needs (“band gap engineering”).

1 these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).

Ternary III-V Alloys (1)The group III lattice sites are occupied by a fraction x of atoms III1 and a fraction (1-x) of atoms III2.

Arsenides: e.g. InGaAs (used in the active regions of high-speed electronic devices, IR lasers, and long-wavelength quantum cascade lasers)

Phosphides: e.g. InGaP (GaAs-based quantum well devices such as red diode lasers)

Antimonides: e.g. AlGaSb (employed in high-speed electronic and infrared optoelectronic devices)

Nitrides: e.g. InGaN (key constituent in the active regions of blue diode lasers and LED’s)

2 these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).

Ternary III-V Alloys (2)The group V lattice sites are occupied by a fraction y of atoms V1 and a fraction (1-y) of atoms V2.

Arsenides Antimonides: e.g. InAsSb (smallest band gap of all III-V’s, very important material for mid-infrared optoelectronic devices)

Arsenides Phosphides: e.g. GaAsP (often used for red LED’s)

Phosphides Antimonides: e.g. GaPSb

Ga these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).xIn1-xP

GaxIn1-xAs

Ternary III-V Alloys (4)Band Gap Engineering: Arsenides, Phosphides, Antimonides

http://www.rpi.edu/~schubert/Light-Emitting-Diodes-dot-org/chap07/F07-06-R.jpg

Ternary III-V Alloys (3) these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).

Band Gap Engineering: Nitrides

l

207 nm

248 nm

http://www.onr.navy.mil/sci_tech/31/312/ncsr/materials/gan.asp

310 nm

413 nm

620 nm

1.24 mm

However: these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).

- More elements → more fabrication issues!!! (e.g. composition control requires tedious calibration growths)
- Range of stable compositions is limited due to the fact that in thermal equilibrium the components of the alloy often tend to segregate into inhomogeneous mixture of binaries and ternaries…

Why?

Provide even greater flexibility in device design…

Quaternary III-V Alloys (2) these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).

The case of GaxIn1-xAsyP1-y

Wide variety of compositions (hence various emission wavelengths) are lattice matched to either GaAs or InP…

Panish, M.B., Temkin, H., Gas source Molecular Beam Epitaxy, Springer, 1993

The misfit is defined as: these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).

as : lattice constant of the substrate material

af : lattice constant of the film material

Design ConsiderationsMost practical devices consists in heterostructures, i.e. layered thin film structures made of dissimilar materials deposited on top of each other (e.g. quantum well). Based on the device requirements, the designer will select the proper alloy, while keeping in mind that typical substrates consist in binary compound (such as GaAs, InP, InP, GaSb) in order to minimize the effects of lattice mismatch.

Lattice-matched structure these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).

By definition, f = 0, i.e. both the substrate material and the film material have the same lattice constant.

A misfit |f| < 5 × 10-4 is generally considered very good, and for practical purposes is assumed lattice-matched (e.g. AlGaAs/GaAs structures)

Ohring, M., The Materials Science of Thin Films, Academic Press, 1992

Strained Structures these bands are actually constituted by N levels of energies (almost a continuum!). The position of upper and lower extreme of each band is however independent of N (depends only on the materials).

f ≠ 0 (i.e. as ≠ af)

f < 0 : compressive strain

f > 0 : tensile strain

For relatively thin film thicknesses, cubic crystals will distort (strain develops within the layer) to achieve the same in-plane lattice constant.

Such a layer is referred to as pseudomorphic.

Ohring, M., The Materials Science of Thin Films, Academic Press, 1992

Burgers vector: atomic displacement needed to generate the dislocation

In the process, defects known as misfit dislocations form at the interface…

Tu, K-N, Mayer, J.W, Feldman, L.C., Electronic thin film science for electrical engineers and materials scientists, McMillan, 1992

Relaxed StructureBeyond a certain critical thickness hc, it is energetically more favourable for the film to “relax”, i.e. achieve a state where its lattice constant tends towards its unstrained value.

Critical Thickness (1) dislocation

hc is obtained by minimizing Etot with respect to the strain. This results in a transcendent equation:

where n is the Poisson’s ratio of the film material.

Mayer, J.W, Lau, S.S., dislocationElectronic Materials Science: For integrated circuits in Si and GaAs, McMillan, 1990

Critical Thickness (2)
Download Presentation

Connecting to Server..